Int. J. Electrochem. Sci., 15 (2020) 7531 – 7544, doi: 10.20964/2020.08.95
International Journal of
Effect of Deformation and Heat Treatment on Pitting Corrosion
Behavior of 7050 Al Alloy
Yao Yao1, Guofeng Li1, Jiaxin Tang1, Wenying Xiong3, Tianqi Chen1, Zhifeng Wang2, Hui Yu2,
1 Department of Mechanical and Electronic Engineering, Changsha University, Changsha 410022, China
2 School of Materials Science and Engineering, Hebei University of Technology, Tianjin 300130, China
3 Hunan Key Laboratory of Advanced Aerospace Materials, Changsha 410205, China
Received: 4 April 2020 / Accepted: 5 June 2020 / Published: 10 July 2020
Microstructure and pitting corrosion behavior of 7050 Al alloy under hot rolling, solution treating and
aging conditions were investigated through optical microscopy, scanning electron microscope,
transmission electron microscope, electrochemical measurements and 3D laser scanning microscope.
The results show the as-rolled alloy exhibits an incomplete recrystallized microstructure with high
dislocation density, while the solution treated alloy presents a complete recrystallized microstructure.
The aging treatment leads to the formation of η' and η precipitates, and AlCuFe intermetallics always
remain in 7050 Al alloy under deformation and heat treatment conditions. The electrochemical activity
increases in the following order: solution-treated alloy < aging-treated alloy < as-rolled alloy, while the
corrosion resistance increases in the reverse order. Potentiostatic polarization test demonstrates that the
as-rolled alloy possesses higher susceptibility to pitting and faster propagation rate. Effects of
microstructure on pitting formation are discussed in detail in this work.
Keywords: 7050 alloy; Pitting Corrosion; Microstructure; Hot rolling; Heat treatment
In the field of aircraft, automobile and rail transit, the weight reduction has always been the goal
that scientists pursue all over the world. Al alloys are dominant in the light weight design of structure
materials because of high strength, excellent processability and low cost . 7050 Al alloy is mainly
alloyed with Zn, Mg and Cu elements, and is a heat treatment strengthening alloy. Through optimizing
the heat treatment to regulate Mg in combination with Zn to form the key strengthening phase MgZn2
(η' or η), 7050 Al alloy can exhibit an ultra-high strength and good fracture toughness [2, 3]. However,
the strength of 7050 Al alloy increases at the expense of decreased corrosion resistance and ductility
Int. J. Electrochem. Sci., Vol. 15, 2020
normally. In addition, 7050 Al alloy products need plastic deformation, such rolling, forging and
extrusion. During the above deformation processes, dislocation, lattice distortion and vacancy are
introduced, which have a hugely detrimental impact on corrosion resistance of 7050 Al alloy. The non-
uniform plastic deformation even causes annulment to subsequent heat treatment . Consequently,
7050 alloy, like other commercial Al alloys, are also faced with problems of pitting corrosion,
intergranular corrosion (IGC), exfoliation corrosion (EXCO) and stress corrosion cracking (SCC) [5-8].
The corrosion types have a heavy dependence on composition, grain structure and precipitates
of Al alloys processed by plastic deformation and heat treatment. The presence of impurities, such as Fe
and Si, usually results in a localized corrosion due to galvanic interaction , thus the control of
elemental impurities can improve corrosion resistance of 7050 alloy. Furthermore, Sun et al.  found
that the more sub-grains were beneficial to the corrosion resistance, while the decrease of the grain size
was adverse. Song et al.  reported that the EXCO resistance of 7050-T6 alloy was improved with
the decreasing quench transfer time and the EXCO susceptibility was significantly affected by the
distribution of precipitates at grain boundaries. Krishnan et al.  developed a novel aging technique
avoiding the loss of solutes at grain boundaries to increase volume fraction of precipitates and to improve
the SCC resistance of 7050 alloy. Hou et al.  used a high-temperature homogenization treatment to
reduce the holding time of 7050 alloy, which also decreased the IGC depth. Actually, pitting corrosion
is regarded as the precarious form of corrosion in Al-alloys [14-16], because it is the initial point of other
corrosion. The trouble is that it cannot be directly detected and predicted by conventional morphology
and electrochemical characterization methods .
In this study, microstructures of 7050 Al alloy under deformation and heat treatment conditions
were observed and investigated. Pitting corrosion behaviors and morphologies of the alloy were
evaluated, and moreover the effect of microstructure on pitting formation was discussed in detail.
2.1. Materials preparation
The as-received 7050 alloy plate with the thickness of 75 mm used in this study was provided by
YUNAN ALUMINUM Co. LTD, and the chemical composition was listed in Table 1. The alloy plate
was subjected to hot rolling at 473℃ to achieve 2 mm sheets. The alloy sheet were solution treated at
540°C for 1h and then quenched in water. Then, the solution-treated sheet was artificial-aged at 125°C
for 24h. As-rolled, solution-treated and aging-treated samples were used for microstructure observation
and electrochemical tests.
Table 1. The chemical composition of as-received 7050 alloy thick plate (wt.%)
Zn Mg Cu Zr Mn Fe Si Al
5.95 2.25 2.1 0.09 0.02 0.06 0.03 Bal.
Int. J. Electrochem. Sci., Vol. 15, 2020
2.2. Microstructure analysis
The microstructure of experimental samples was observed by optical microscopy (OM, MJ42,
Mshot), scanning electron microscope (SEM, Hitachi, SU1500) and transmission electron microscope
(TEM, FEI, Tecnai G2 20). For OM observation, the samples under conditions were ground and
polished, then etched with a Keller reagent. The samples for SEM observation were ground and polished,
then cleaned directly with absolute ethyl alcohol in an ultrasonic cleaning machine. The samples for
TEM analysis were mechanically ground to a thickness of 80 µm and then thinned by twin-jet
electropolishing with the solution of 25% nitric acid and 75% methyl alcohol at -25°C.
2.3. Electrochemical measurements
Electrochemical tests were performed by an Adminal electrochemical system (Squidstat Plus,
USA) with the typical three electrode comprised of an Ag/AgCl electrode as the reference electrode, a
platinum plate with a dimension of 4 × 4 × 0.2mm as the counter electrode, and 1 cm2 of the alloy as the
working electrode. All tests used 0.001 mol·L-1 NaCl solution as the electrolyte. Open circuit potentials
(OCP) were achieved after an immersion in the electrolyte for 30 min. Potentiodynamic polarization
tests were carried out and the testing range from -200 mV to 600 mV with respect to OCP at a scanning
rate of 1 mV·s-1. After the samples were immersed in the electrolyte for achieving a stable OCP,
electrochemical impedance spectroscopy (EIS) was measured at the OCP from 100 kHz to 0.05 Hz with
the voltage amplitude of 5 mV.
2.4 Pitting corrosion behavior evaluation
The three electrode system was also employed to evaluate pitting corrosion behaviors of
experimental samples. To improve the detection precision, the samples were ground with emery 5000
grit papers, then were polished and cleaned with absolute ethyl alcohol. Potentiostatical polarization
tests were used at -600mV (vs Ag/AgCl) for 300 min. Furthermore, the corroded surfaces were estimated
with a 3D laser scanning microscope (Keyence VK-X100, Keyence, Japan). The morphology, number,
depth, area and volume of pits were systematically analyzed.
3. RESULTS AND DISCUSSION
The optical microstructures of 7050 alloy under different conditions are illustrated in Fig. 1. For
the as-rolled alloy, elongated and recrystallized grains are observed in Fig. 1a. Due to the effect of heat
and deformation force, dynamic recovery and recrystallization occur in the alloy during the hot rolling.
Fig. 1b shows coarse grains implying that the solution treated alloy is recrystallized completely and then
grains grow up. After the aging treatment, it difficult to identify the grain structure, while the
Int. J. Electrochem. Sci., Vol. 15, 2020
precipitation of secondary phases is obviously viewed in consideration of numerous black particles on
Fig.1c. In order to better distinguish impurities, Fig. 2 gives backscattered electron (BSE) images of
experimental samples. Obviously, the alloys in different states contain similar intermetallics. Moreover,
the major elements including Al, Cu and Fe are detected by